Origins of 1/f noise in nanostructure inclusion polymorphous silicon films
 Shibin Li^{1, 2},
 Yadong Jiang^{1},
 Zhiming Wu^{1}Email author,
 Jiang Wu^{2},
 Zhihua Ying^{3},
 Zhiming Wang^{2}Email author,
 Wei Li^{1} and
 Gregory Salamo^{2}
DOI: 10.1186/1556276X6281
© Li et al; licensee Springer. 2011
Received: 18 December 2010
Accepted: 4 April 2011
Published: 4 April 2011
Abstract
In this article, we report that the origins of 1/f noise in pmSi:H film resistors are inhomogeneity and defective structure. The results obtained are consistent with Hooge's formula, where the noise parameter, α _{H}, is independent of doping ratio. The 1/f noise power spectral density and noise parameter α _{H} are proportional to the squared value of temperature coefficient of resistance (TCR). The resistivity and TCR of pmSi:H film resistor were obtained through linear currentvoltage measurement. The 1/f noise, measured by a custombuilt noise spectroscopy system, shows that the power spectral density is a function of both doping ratio and temperature.
Introduction
Nanostructure semiconductor has been the focus of intense interest in recent years due to their extensive device application [1–6]. It is well known that hydrogenated polymorphous silicon is a nanostructure inclusion material [7–9]. Hydrogenated silicon films commonly exhibit high noise at low frequency (f). This noise has a spectral power density of the type S(f) ∝ 1/f ^{ a }, where a is known as "1/f noise." However, lower noise materials are important for highperformance semiconductor devices. 1/f noise of amorphous and polycrystalline silicon has captured the attention of researchers in the field of electronics and physics for several decades [10]. Polymorphous silicon film is generally prepared by operating a strong hydrogendiluted silane plasma source at high pressure and power density [11]. Many efforts have been made concerning the growth process, microstructure, transport, and optoelectronic properties of pmSi:H films [12]. The results indicate that pmSi:H films show higher transport properties than aSi:H, a highly desirable trait for the production of devices, such as solar cells and thin film transistors. To date, pmSi:H investigations have focused on certain applications, but there is no study devoted to the 1/f noise of such materials except those by our group which have reported the dependence of 1/f noise on the change of material structure of silicon films [13–15]. In this article, we focus on the study of the origins of 1/f noise in pmSi:H and investigate the influence of boron doping ratio on 1/f noise in pmSi:H films.
Experimental
Results and discussions
Structure and electrical properties for different doping ratios in pmSi:H film
Sample  R _{v}  h(nm)  R _{0}(MΩ)  N _{C}  β(%)  X _{C}(%)  H(%)  Void (%) 

A  10^{2}  326  2.42  4.24 × 10^{14}  2.78  20  18  0 
B  10^{3}  335  4.53  3.54 × 10^{13}  2.93  18  16  0.5 
C  10^{4}  341  6.76  4.23 × 10^{12}  3.28  17  15  0.8 
D  10^{5}  352  8.21  3.85 × 10^{11}  3.45  14  13  1 
where S _{v} is the noise power density at voltage V, α _{H} is the noise parameter, f is frequency, and N _{C} is the total number of charge carriers in a certain volume involved in noise generation. The total number of charge carriers, determined by Hall measurement, in conjunction with the dimension of the pmSi:H film resistor, determines the noise parameter α _{H} as a function of frequency. Our experimental results also demonstrate the 1/f noise power scales with the square of bias voltage, which is in agreement with the results of Fine et al. [17].
For each measured sample here, the values of N _{C}, f, and V ^{2} are constant. The value of noise parameter α _{H} at 100 Hz is plotted against temperature for different doping ratios as shown in the inset of Figure 5b. The noise parameter α _{H} for the pmSi:H film resistors in this study is also a function of the squared TCR (α_{H} ∝ β^{2}). It demonstrated that the resistance fluctuation of the film samples also resulted in the variation of noise parameter when the measurement temperature changed dramatically.
Conclusions
The results of this study demonstrated that the origins of 1/f noise in nanostructure inclusion pmSi:H are the inhomogeneity and the defective structure in the films. The power spectral density of 1/f noise is inversely proportional to boron doping ratio, which is consistent with Hooge's formula. The value of S _{v}/V ^{2} is constant when the voltage is less than 1 V, demonstrating that resistance fluctuation is not the origin of 1/f noise in pmSi film resistors in the case of constant temperature. At 100 Hz, the temperature dependence of 1/f noise indicates that the power spectral density and the noise parameter α _{H} are proportional to the squared TCR. It has also been proven that the resistance fluctuation of the film samples also results in the variation of noise parameter when the measurement temperature changed dramatically.
Abbreviations
 TCR:

temperature coefficient of resistance.
Declarations
Acknowledgements
This work was partially supported by National Science Foundation of China via grant No. 60901034 and 60425101.
Open access
This article is distributed under the terms of the Creative Commons Attribution Noncommercial License which permits any noncommercial use, distribution, and reproduction in any medium, provided the original author(s) and source are credited.
Authors’ Affiliations
References
 Li SS, Xia JB: Electronic structure of a hydrogenic acceptor impurity in semiconductor nanostructures. Nanoscale Res Lett 2007, 2: 554. 10.1007/s1167100790989View Article
 Arendse CJ, Malgas GF, Muller TFG, Knoesen D, Oliphant CJ, Motaung DE, Halindintwali S, Mwakikunga BW: Thermally induced nanostructural and optical changes of ncSi:H deposited by hotwire CVD. Nanoscale Res Lett 2009, 4: 307. 10.1007/s1167100892430View Article
 Li SS, Xia JB: Linear Rashba model of a hydrogenic donor impurity in GaAs/GaAlAs quantum wells. Nanoscale Res Lett 2009, 4: 178. 10.1007/s1167100892225View Article
 Li SB, Han L, Chen Z: The interfacial quality of HfO _{ 2 } on silicon with different thicknesses of the chemical oxide interfacial layer. J Electrochem Soc 2010, 157: G221. 10.1149/1.3483789View Article
 Li SS, Xia JB: Electronic structures of GaAs/AlxGa1xAs quantum double rings. Nanoscale Res Lett 2006, 1: 167. 10.1007/s116710069010zView Article
 Zhou M, Zhou JY, Li RS, Xie EQ: Preparation of aligned ultralong and diameter controlled silicon oxide nanotubes by plasma enhanced chemical vapor deposition using electrospun PVP nanofiber template. Nanoscale Res Lett 2010, 5: 279. 10.1007/s1167100994766View Article
 Voyles PM, Gerbi JM, Treacy MMJ, Gibson JM, Abelson JR: Absence of an abrupt phase change from polycrystalline to amorphous in silicon with deposition temperature. Phys Rev Lett 2001, 86: 5514. 10.1103/PhysRevLett.86.5514View Article
 Chaâbane N, Kharchenko AV, Vach H, Roca i Cabarrocas P: Optimization of plasma parameters for the production of silicon nanocrystals. New J Phys 2003, 5: 37.1.View Article
 Fontcuberta i Morral A, Roca i Cabarrocas P, Clerc C: Structure and hydrogen content of polymorphous silicon thin films studied by spectroscopic ellipsometry and nuclear measurements. Phys Rev B 2004, 69: 125307. 10.1103/PhysRevB.69.125307View Article
 Yoon HP, Yuwen YA, Kendrick CE, Barber GD, Podraza NJ, Redwing JM, Mallouk TE, Wronski CR, Mayer TS: Enhanced conversion efficiencies for pillar array solar cells fabricated from crystalline silicon with short minority carrier diffusion lengths. Appl Phys Lett 2010, 96: 213503. 10.1063/1.3432449View Article
 Li SB, Wu ZM, Jiang YD, Yu JS, Li W, Liao NM: Growth mechanism of microcrystalline and polymorphous silicon film with pure silane source gas. J Phys D 2008, 41: 105207. 10.1088/00223727/41/10/105207View Article
 Butté R, Vignoli S, Meaudre M, Meaudre R, Marty O, Saviot L, Roca i Cabarrocas P: Plasma enhanced chemical vapor deposition of amorphous, polymorphous and microcrystalline silicon films. J NonCryst Solids 2000, 266–269: 263.View Article
 Li SB, Wu ZM, Jiang YD, Li W, Liao NM, Yu JS: Structure and 1/f noise of boron doped polymorphous silicon films. Nanotechnology 2008, 19: 085706. 10.1088/09574484/19/8/085706View Article
 Li SB, Wu ZM, Li W, Liao NM, Yu JS, Jiang YD: Influence of microcrystallization on noise in borondoped silicon film. Phys Status Solidi A 2007, 204: 4292. 10.1002/pssa.200723235View Article
 Li SB, Wu ZM, Jiang YD, Li W, Liao NM, Yu JS: Noise in boron doped amorphous/microcrystallization silicon films. Appl Surf Sci 2008, 254: 3274. 10.1016/j.apsusc.2007.11.004View Article
 Hooge FN: 1/f noise is no surface effect. Phys Lett A 1979, 29: 139. 10.1016/03759601(69)900760View Article
 Fine BV, Bakker JPR, Dijkhuis JI: Longrange potential fluctuations and 1/ f noise in hydrogenated amorphous silicon. Phys Rev B 2003, 68: 125207. 10.1103/PhysRevB.68.125207View Article
 NguyenTran T, Suendo V, Roca i Cabarrocas P, Nittala LN, Bogle SN, Abelson JR: Fluctuation microscopy evidence for enhanced nanoscale structural order in polymorphous silicon thin films. J Appl Phys 2006, 100: 094319. 10.1063/1.2360381View Article
 Paul AWE, Dijkhuis JI: Resistance fluctuations in hydrogenated amorphous silicon: Thermal equilibrium. Phys Rev B 1998, 58: 3904. 10.1103/PhysRevB.58.3904View Article
 Voss RF, Clark J: Flicker (1/ f ) noise: equilibrium temperature and resistance fluctuations. Phys Rev B 1976, 13: 556. 10.1103/PhysRevB.13.556View Article
Copyright
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.